Series of Novel 3D Heterometallic Frameworks Based on the Co(II) Coordination Chains and Ln(III) Coordination Layers
Liao, Sheng-Yun; Gu, Wen; Yang, Lin-Yan; Li, Tian-Hao; Tian, Jin-Lei; Wang, Li; Zhang, Ming; Liu, Xin; Crystal Growth & Design 12 (2012) 3927–; doi:10.1021/cg300326e

data_4506449
_publ_section_title
;
 Series of Novel 3D Heterometallic Frameworks Based on the Co(II)
 Coordination Chains and Ln(III) Coordination Layers
;
_journal_issue                   8
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              3927
_journal_paper_doi               10.1021/cg300326e
_journal_volume                  12
_journal_year                    2012
_chemical_formula_sum            'C40 H28 Co N12 O20 Tb2'
_chemical_formula_weight         1373.51
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                84.041(2)
_cell_angle_beta                 84.911(2)
_cell_angle_gamma                62.580(2)
_cell_formula_units_Z            1
_cell_length_a                   9.1880(9)
_cell_length_b                   10.6721(10)
_cell_length_c                   12.6208(12)
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      54.96572
_cell_measurement_theta_min      6.088577
_cell_volume                     1091.40(18)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71075
_diffrn_reflns_av_R_equivalents  0.0376
_diffrn_reflns_av_sigmaI/netI    0.0556
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            7109
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         3.04
_exptl_absorpt_coefficient_mu    3.681
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.6533
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    2.090
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             669
_exptl_crystal_size_max          0.30
_exptl_crystal_size_mid          0.28
_exptl_crystal_size_min          0.25
_refine_diff_density_max         0.936
_refine_diff_density_min         -1.124
_refine_diff_density_rms         0.180
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.152
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     352
_refine_ls_number_reflns         3829
_refine_ls_number_restraints     8
_refine_ls_restrained_S_all      1.151
_refine_ls_R_factor_all          0.0471
_refine_ls_R_factor_gt           0.0400
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0565P)^2^+0.1453P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0929
_refine_ls_wR_factor_ref         0.1040
_reflns_number_gt                3489
_reflns_number_total             3829
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg300326e_si_009.cif
_cod_data_source_block           c110322c
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               4506449